This content has been downloaded from IOPscience. Please scroll down to see the full text.
IP Address: 184.108.40.206
This content was downloaded on 07/10/2014 at 11:15
Please note that terms and conditions apply.
Anomalous glass transition behavior of SBR–Al2O3 nanocomposites at small filler
View the table of contents for this issue, or go to the journal homepage for more 2014 Nanotechnology 25 425704
Anomalous glass transition behavior of
nanocomposites at small
Rymma Sushko, Marlena Filimon, Rick Dannert, Patrick Elens,
Roland Sanctuary and Jörg Baller
Physics and Materials Science Research Unit, Laboratory for the Physics of Advanced Materials, University of Luxembourg, 162A avenue de la Faїencerie, L-1511, Luxembourg
Received 12 May 2014, revised 8 August 2014 Accepted for publication 28 August 2014 Published 3 October 2014
Elastomersﬁlled with hard nanoparticles are of great technical importance for the rubber industry. In general,ﬁllers improve mechanical properties of polymer materials, e.g. elastic moduli, tensile strength etc. The smaller the size of the particles, the larger is the interface where interactions between polymer molecules andﬁllers can generate new properties. Using temperature-modulated differential scanning calorimetry and dynamic mechanical analysis, we investigated the properties of pure styrene-butadiene rubber (SBR) and SBR/alumina
nanoparticles. Beside a reinforcement effect seen in the complex elastic moduli, small amounts of nanoparticles of about 2 wt% interestingly lead to an acceleration of the relaxation modes responsible for the thermal glass transition. This leads to a minimum in the glass transition temperature as a function of nanoparticle content in the vicinity of this critical concentration. The frequency dependent elastic moduli are used to discuss the possible reduction of the
entanglement of rubber molecules as one cause for this unexpected behavior.
Keywords: nanocomposites, styrene-butadiene, alumina, nanoparticles, glass transition, DMA, TMDSC
(Someﬁgures may appear in colour only in the online journal)
Nowadays, many research works are dedicated to the mod-iﬁcation of polymer properties using nanometer sized ﬁllers [1, 3, 13, 16, 28, 30]. The improvement of mechanical properties of polymers [13,14,16,18,29,30] is important for many applications, e.g. reinforcement of elastomers  for the use in car tires. Inﬁlled polymers, the mobility of polymer molecules is often reduced. This can be due to e.g. con ﬁne-ment effects by the ﬁllers or due to interactions between polymer molecules andﬁller particles. This effect is usually
more pronounced for nanometer sized ﬁllers than for micrometer sized ﬁllers [28, 30]. The reduced mobility often leads to increased glass transition temperatures [7, 10, 19–21, 23, 26]. The introduction of ﬁllers into a polymer matrix is generally accompanied by the formation of layers (interphases) of slowed molecular dynamics around the particles [2, 9, 12, 25, 26]. In elastomers, interphases with almost immobile molecules are known as bound rubber . If the difference in mobility between molecules in the inter-phase and the bulk is high enough, two glass transitions have also been reported [2,25,26]. Depending on the interaction between ﬁllers and matrix molecules, unchanged [5, 22] or even accelerated  molecular dynamics can be found too (for a decent review please see ). The sign of the ﬁller inﬂuence on the mobility of polymer molecules may even depend on the molecular weight of the matrix molecules . Nanotechnology 25 (2014) 425704 (8pp) doi:10.1088/0957-4484/25/42/425704
Most of the studies analyze the effect of high nanoparticle concentrations up to 50 wt% on the composites’ properties. Nevertheless, even at smallﬁller contents, changed molecular mobility leading to changes in the glass transition behavior has been reported [8–10]. With the exception of the work of Bindu et al , it is common for all studies cited above, that the incorporation of nanoparticles inﬂuences the glass tran-sition temperatures for a given system only in one way (increase, decrease or no change). In the present work, we present a system (styrene-butadiene rubber (SBR)ﬁlled with untreated alumina nanoparticles) where both accelerated as well as reduced molecular dynamics can be found for the same system. This leads to a minimum in the glass transition temperature at small ﬁller concentrations. Dynamic mechan-ical analysis (DMA), rheometry and temperature-modulated differential scanning calorimetry (TMDSC) together with structural investigation tools have been used to shed light on this unexpected experimentalﬁnding.
2. Experimental 2.1. Materials
Poly(styrene-co-butadiene) rubber (SBR, Sigma-Aldrich) con-taining 45% of styrene and alumina nanoparticles (Aeroxide Alu C delivered by Evonik) were used in this work. According to the producer, the average diameter of the primary particles produced by noble gas condensation is about 13 nm. During the production process, primary particles sinter into irregularly shaped, chemically bonded aggregates. This leads to fractal nanoparticles with linear dimensions between 13 and 200 nm . The solvent used in this work (chloroform) is of spectro-scopic purity grade, supplied by Carl Roth GmbH.
2.2. Composite preparation and characterization
To produce the SBR/AluC nanocomposites, the following procedure was used : a known mass of AluC nanoparticles was dispersed and sonicated in chloroform, after which a known quantity of 10% SBR solution in chloroform was injected. This mixture was stirred in a planetary mixer for 15 min and then freeze–dried. The samples for investigations were molded into disks in a vacuum oven at 85 °C during 24 h. Thus, a series of disk-like nanocomposites containing 1, 1.5, 2, 3, 4, 10 and 20 wt% of AluC nanoparticles was pre-pared. To examine the dispersion of the alumina nanoparticles in the SBR matrix, cross-section samples were cut using a microtome. The cross-sectioned areas were examined by transmission electron microscopy (TEM). The TEM (JEOL JEM 2011-HRTEM) was operated at an acceleration voltage of 100 kV. Figure 1 shows TEM pictures of SBR samples ﬁlled with 1, 2 and 4 wt% of alumina nanoparticles at four different magniﬁcations. The highest magniﬁcation of the 1% sample depicts the chemical aggregation of the primary par-ticles (13 nm) to fractal nanoparpar-ticles (up to 200 nm in dia-meter). It has been shown that these aggregates cannot be broken even by high shear forces . The higher
concentrations (2% and 4%) show the formation of small agglomerates of aggregates. Prior investigations have shown  that these agglomerates can easily be broken by applying shear forces, e.g. in AluC/epoxy resin nanocomposites. Therefore we assume that the agglomerates are held together by small Van der Waals forces due to the hydrophilic nature of the aluminas’ surfaces.
To ensure the rightﬁller concentrations especially at low ﬁller contents, degradation experiments between 300 and 770 K were performed using thermogravimetric analysis (TGA, TA Instruments TGA 2590) (ﬁgure2).
Temperature-modulated differential scanning calorimetry (TMDSC, Mettler Toledo DSC 823) was used to investigate the glass transition behavior of the SBR nanocomposites. Samples of 6–10 mg were weighed and sealed in aluminum pans. TMDSC measurements were performed in nitrogen atmosphere in the temperature range from 298 to 223 K with a cooling rate of 0.5 K min−1, a temperature modulation amplitude of 0.5 K and a modulation period of 2 min. The real and imaginary parts of the speciﬁc heat capacity were eval-uated using standard methods . The glass transition temperature was determined as the inﬂection point of the real part of the speciﬁc heat capacity. Temperature and heat ﬂow calibration of the calorimeter was done using adamantane, water, indium, naphthalene, benzoic acid and zinc standards. The viscoelastic behavior of the samples was character-ized at low strains (linear regime conditions) using DMA (Mettler Toledo DMA/SDTA 861e). Two equal disks of each nanocomposite with diameters of about 8 mm and thicknesses of about 1 mm were mounted into a shearing device. The storage G′ and loss G″ parts of the dynamic shear modulus were isothermally measured as a function of frequency (from 0.008 to 800 Hz) at the following temperatures: 223, 233, 243, 253, 273, 293, 313, 333, 353 and 373 K. The DMA method is limited by the fact that the sample holder can only poorly be adapted to the changing thickness of the sample. This holds especially true at low temperatures (high fre-quencies in the master curves) near or below the thermal glass transition. To overcome this problem, rheometry (Anton Paar MCR 302 rheometer) was also performed on disc-like sam-ples in parallel plate geometry (diameter 8 mm). For more details of the experimental setup see . During the rheo-logical measurements, the normal force was kept constant at 2 N and the gap size (usually between 1 and 2 mm) was allowed to adapt to the thermal expansion of the samples. Using this conﬁguration, we were able to measure loss curves (tanδ) in the region of the dynamic glass transition (ﬁgure9). The rheology measurements were made by isothermal fre-quency sweeps at 238, 243, 248, 253, 263, 273, 283, 288, 303, 303, 323 and 343 K. The measurement conditions were always chosen to strictly respect the linear response regime for each frequency f and at any given temperature T. 2
3. Results and discussion 3.1. Results from calorimetry
The upper part of ﬁgure 3 shows the glass transition tem-peratures Tgof the SBR/Alu C composites for differentﬁller
concentrations. The most prominent feature is an unexpected minimum in Tgat wAluC≈ 1.5–2 wt%.
The slight increase of Tgfrom the pure SBR system to the
systemﬁlled with 20 wt% of alumina nanoparticles measures up to expectations: (i) the mere presence of the nanoparticles hinders the ﬂow/movement of the polymer molecules, (ii) interactions between SBR molecules and the nanoparticles’ surfaces are expected to slow down the molecular dynamics of the composite system. As the change of Tgremains small
for highﬁller loading (wAluC> 10 wt%), it can be suggested
that the molecular mobility of the chains is only moderately slowed down by the new interactions promoted between the
hydrophilicﬁllers and the hydrophobic matrix molecules. The unexpected minimum in Tg signiﬁes an acceleration of the
dynamics of the SBR molecules for lowﬁller concentrations compared to the pure SBR system.
3.2. Results from mechanical spectroscopy
Dynamic mechanical investigations were conducted to examine the effect of nanoﬁllers on the thermomechanical properties of SBR nanocomposites. Figure 4 shows master curves of the storage modulus G′(f) and loss modulus G″(f) for composites with different concentrations of alumina nanoparticles. As an overview, ﬁgure4 shows the effect of the incorporation of nanoparticles on the G′ and G″ curves for the systems containing 0%, 10% and 20% Alu C. These systems obviously present noticeable reinforcement effect. The master curves (ﬁgure 4) display four different regions which are characteristic for the viscoelastic behavior of
rubber-like materials: (i) the glassy region in the high fre-quency range where the composites are dynamically frozen; (ii) the transition zone between glass and rubber where the mechanic properties are dominated by the structural relaxa-tion processes connected to the dynamic freezing; (iii) the rubbery plateau where the slope of the master curves is reduced due to physical cross-links by entanglement of SBR molecules; (iv) the terminalﬂow range at low frequencies.
Figure5shows the inﬂuence of the nanoparticles on the elastic moduli in the region around the rubbery plateau in more detail. To construct the master curves for a reference
temperature of 273 K, the temperature–frequency equivalence principle has been exploited. The corresponding horizontal shift factors log aTfor all nanocomposite systems are depicted
inﬁgure6. No vertical shift was necessary (bT= 1). The shape
of the log aTcurves does not vary much with the nanoparticle
content. This means that the temperature dependencies of the intrinsic relaxation processes are qualitatively the same for all nanoparticle concentrations.
In the glassy region, the effect of the nanoparticles is less pronounced than in the other regions. This is due to the fact that the stiffness moduli of the SBR matrix approach the high moduli of the alumina nanoparticles at high frequencies. In all other regions, the reinforcement effect of the nanoparticles can clearly be seen in the frequency dependency of both master curves.
The reinforcement effect is also found for small nano-particle concentrations below 10 wt%, butﬁgure5shows that there is a dependency of this effect on the probe frequency. Figures7and8resolve this dependency for both the real part (ﬁgure7) as well as for the imaginary part (ﬁgure8) of the complex elastic modulus measured by DMA.
The G′(wAluC) curve for 10−4Hz shows a reinforcement
effect which increases with the concentration of nano-particles. This general trend is observed up to a frequency of about 10 Hz. For higher frequencies approaching the dynamic glass transition, the reinforcement increases rapidly at low concentrations—almost showing a maximum at about wAluC= 1.5 wt%. The same behavior can be observed for the
G″(wAluC) curves. The maximum at about wAluC= 1.5 wt% is
even more pronounced. Comparing the concentration dependency of both moduli with theﬁller content dependency of the thermal glass transition temperature (ﬁgures7and8), it turns out that the maximum in the moduli is found at the same nanoparticle concentration as the minimum in Tg.
The most prominent feature of the presented experimental results is the minimum in the glass transition temperature Tg
of the nanocomposites for low ﬁller concentrations. This minimum is accompanied by a general trend towards increasing Tgvalues with increasing nanoparticle
concentra-tion. It can only be explained by a mechanism or process which accelerates the dynamics of the rubber molecules for ﬁller concentrations up to about 2 wt%. This would be the opposite of what is known as ‘bound rubber’ . Since the untreated alumina nanoparticles have a hydrophilic character, it could be argued that the hydrophobic rubber molecules show only weak interactions with the nanoparticles’ surfaces leading to accelerated dynamics of rubber molecules near nanoparticle surfaces. This should however also be the case for higher ﬁller concentrations leading to a general trend to lower glass transition temperatures which is at ﬁrst sight in contradiction to the experimental ﬁndings. However, Bindu et al  argue for natural rubber/ZnO nanocomposites that, starting at concentrations of about 2 vol%, aggregation of nanoparticles takes place leading to a preference of nano-particle/nanoparticle interactions over nanoparticle/rubber
Figure 2.Experimental AluC concentration wAluCdetermined by
thermogravimetry versus theoretical AluC concentration for the nanocomposites under study.
Figure 3.Glass transition temperatures Tgfrom the real part of the
speciﬁc heat capacity (measured at 8.3 mHz with TMDSC) and frequency positions of the maxima of the tanδ curves (at 273 K from rheology,ﬁgure9) as a function of nanoparticle content.
interactions. Our TEM data (ﬁgure1) shows a slight tendency for the nanoparticles to cluster, but this tendency can be found for all of the samples investigated by TEM (1%, 2% and 4%). The sample with 2% does not show any peculiarities. Fur-thermore, experiments with SBR nanocomposites with the same alumina particles but coated with several different hydrophobic layers (to be published) show a similar Tg
minimum at low ﬁller concentrations. This leads us to the conclusion that aggregation of nanoparticles is not the reason for the observed behavior. Moreover we claim that the reduction of the number of entanglements (physical cross-links) between polymer chains by the presence of small amounts of nanoparticles is responsible for the accelerated local dynamics at small ﬁller concentrations. During the preparation of the nanocomposites from solution, the nano-particles seem to hinder the formation of physical cross-links. The structural relaxation (α-process) of the SBR molecules becomes faster which explains the decrease of Tg for these
small concentrations. Since the number of entanglements in unﬁlled SBR rubber is limited, there is also a limit for the acceleration of the molecular dynamics. The accelerated dynamics at low concentrations is superimposed by a general trend to lower local dynamics with increasing ﬁller con-centration. This could be due to the fact that interactions at the nanoparticles’ surfaces have a small retardation effect on the glass forming dynamics of the SBR molecules. This effect seems to be far too small to talk of ‘bound rubber’: the increase of Tgfrom unﬁlled to 20 wt% is only about 1.7 K! In
addition to possible attractive interactions between rubber molecules and nanoparticle surfaces, conﬁnement of the rubber molecules by the presence of the nanoparticles could also be the reason for the slight overall increase of the glass transition temperature.
Measurements of the loss factor tanδ by rheology support the idea of increased (at about 1.5–2%) and slowed (>4%) mobility: in the upper part ofﬁgure9, the frequency dependence of tanδ at a reference temperature of 273 K is shown. The lower part shows the same curves scaled ver-tically by a factor in a way that all curves have the same height at the maximum. There are two important results: (i) The shift of a single tanδ curve with a speciﬁc nanoparticle concentration with regard to the curve of the unﬁlled rubber is the same at all frequencies shown inﬁgure9. This means that the inﬂuence of the nanoparticles on the dynamics of the rubber molecules is the same for low frequencies where ﬂow plays a major role and for high frequencies around the dynamic glass transition temperature where segmental mobility dominates. This holds true for the curves which are shifted to higher frequencies as well as for curves shifted to lower frequencies. (ii) The shift of the tanδ maximum with the concentration of the nanoparticles, i.e. the dynamic glass transition at the reference temperature of 273 K, reﬂects the results of the TMDSC measurements: in the lower part of ﬁgure 3, the frequencies of the tanδ maximum are plotted as a function ofﬁller content. At the concentrations where the Tgvalues show a minimum, the
tanδ data shows a maximum. Using the activation plot of the α-process measured by dielectric spectroscopy for the pure SBR system, it can be calculated that the 8.3 mHz at Tg from the TMDSC measurements corresponds to about
300 Hz at the reference temperature of 273 K used for the master curves of the tanδ data. From the fact, that the concentration dependent shift of the tanδ curves is inde-pendent of the frequency (see (i)), it can be expected that the Tgminimum from TMDSC measurements can be found
at the same nanoparticles concentration as the maximum of the tanδ curves.
To summarize, acceleration due to reduction of entan-glements on one hand and retardation due to nanoparticle/ rubber interactions and conﬁnement on the other hand are made responsible for the unexpected behavior of the glass transition temperature from TMDSC and the loss maximum from rheology.
The effect of the disentanglement can be seen in both moduli (ﬁgures7and8): there is a step atﬁller concentrations where the inﬂuence of disentanglement is expected to end.
Nanocomposites of untreated alumina nanoparticles and uncured SBR rubber were prepared and their thermal and
Figure 5.Master curves of the elastic moduli of all nanocomposites in a frequency region around the rubbery plateau. DMA measurements, reference temperature: 273 K.
Figure 6.Horizontal shift factors log aTused to construct the master
curves displayed inﬁgures4and5. DMA measurements, reference temperature: 273 K.
Figure 7.Storage modulus G′ (DMA measurements) as a function of nanoparticle content, evaluated at different frequencies at the reference temperature of 273 K. Lines are guides for the eyes. The uppermost curve on the left side shows the dependency of the glass transition temperature of the nanoparticle content as measured by TMDSC.
dynamic mechanical properties were investigated by calorimetry and mechanical spectroscopy. An unexpected minimum in the glass transition temperature at small ﬁller concentrations could be found. Two opposed processes are made responsible for the observed behavior: the underlying trend to higher glass transition temperatures with higher nanoparticle content is attributed to weak nanoparticle/ rubber interactions and to conﬁnement effects. Acceleration of molecular dynamics is considered as being a con-sequence of a reduction of the number of entanglements due to the presence of the nanoparticles during sample pre-paration from solution. This accelerating inﬂuence is lim-ited by the total amount of entanglements present in the neat SBR. More investigations with different surface treatments of the nanoparticles are under way. First results conﬁrm the presented minimum of the glass transition temperature for all of these systems. In our view, this supports the inter-pretation of the acceleration of the structural relaxation process being a consequence of disentanglement caused by the nanoparticles.
This work was kindly supported by the Fonds National de la Recherche Luxembourg. We thank Jörg Schmauch from the Universität des Saarlandes, Germany, for support with the
TEM measurements. We thank the Goodyear Innovation Center Luxembourg for continuing support.
 Alexandre M and Dubois P 2000 Polymer-layered silicate nanocomposites: preparation, properties and uses of a new class of materials Mater. Sci. Eng.28 1–63
 Arrighi V, McEwen I J, Qian H and Prieto M B S 2003 The glass transition and interfacial layer in styrene-butadiene rubber containing silica nanoﬁller Polymer44 6259–66
 Balazs A C, Emrick T and Russell T P 2006 Nanoparticle polymer composites: where two small worlds meet Science
 Ballav N and Biswas M 2003 Preparation and evaluation of a nanocomposite of polythiophene with Al2O3Polym. Int.52
 Baller J, Becker N, Ziehmer M, Thomassey M, Zielinski B, Müller U and Sanctuary R 2009 Interactions between silica nanoparticles and an epoxy resin before and during network formation Polymer50 3211–9
 Baller J, Thomassey M, Ziehmer M and Sanctuary R 2011 The catalytic inﬂuence of alumina nanoparticles on epoxy curing Thermochim. Acta517 34–9
 Baller J, Thomassey M, Ziehmer M and Sanctuary R 2011 Thermoplastic and Thermosetting Polymers and Composites
Figure 8.Loss modulus G″ (DMA measurements) as a function of
nanoparticle content, evaluated at different frequencies at the reference temperature of 273 K. Lines are guides for the eyes. The uppermost curve on the left side shows the dependency of the glass transition temperature of the nanoparticle content as measured by TMDSC.
ed L D Tsai and M R Hwang (Hauppauge: Nova Science Publishers) 197–212
 Bansal A, Yang H, Li C, Benicewicz R C, Kumar S K and Schadler L S 2006 Controlling the thermornechanical properties of polymer nanocomposites by tailoring the polymer–particle interface J. Polym. Sci. B44 2944–50  Bansal A, Yang H C, Li C Z, Cho K W, Benicewicz B C,
Kumar S K and Schadler L S 2005 Quantitative equivalence between polymer nanocomposites and thin polymerﬁlms Nat. Mater.4 693–8
 Bindu P and Thomas S 2013 Viscoelastic behavior and reinforcement mechanism in rubber nanocomposites in the vicinity of spherical nanoparticles J. Phys. Chem. B117
 Cangialosi D, Boucher V M, Alegria A and Colmenero J 2013 Physical aging in polymers and polymer nanocomposites: recent results and open questions Soft Matter9 8619–30  Ciprari D, Jacob K and Tannenbaum R 2006 Characterization
of polymer nanocomposite interphase and its impact on mechanical properties Macromolecules39 6565–73  Coleman J N, Khan U and Gun’ko Y K 2006 Mechanical
reinforcement of polymers using carbon nanotubes Adv. Mater.18 689–706
 Daniel I M, Miyagawa H, Gdoutos E E and Luo J J 2003 Processing and characterization of epoxy/clay
nanocomposites Exp. Mech.43 348–54  Dannert R, Sanctuary R, Thomassey M, Elens P,
Krüger J K and Baller J 2014 Strain-induced low-frequency relaxation in colloidal DGEBA/SiO2 suspensions Rheolo. Acta doi:10.1007/s00397-014-0788-9
 Evora V M F and Shukla A 2003 Fabrication, characterization, and dynamic behavior of polyester/TiO2nanocomposites
Mater. Sci. Eng. A361 358–66
 Gauthier C, Reynaud E, Vassoille R and Ladouce-Stelandre L 2004 Analysis of the non-linear viscoelastic behaviour of silicaﬁlled styrene butadiene rubber Polymer45 2761–71  Guo Z H, Pereira T, Choi O, Wang Y and Hahn H T 2006
Surface functionalized alumina nanoparticleﬁlled polymeric nanocomposites with enhanced mechanical properties J. Mater. Chem.16 2800–8
 Heinrich G, Kluppel M and Vilgis T A 2002 Reinforcement of elastomers Curr. Opin. Solid State Mater. Sci.6 195–203
 Lee A and Lichtenhan J D 1998 Viscoelastic responses of polyhedral oligosilsesquioxane reinforced epoxy systems Macromolecules31 4970–4
 Priestley R D, Rittigstein P, Broadbelt L J, Fukao K and Torkelson J M 2007 Evidence for the molecular-scale origin of the suppression of physical ageing in conﬁned polymer: ﬂuorescence and dielectric spectroscopy studies of polymer–silica nanocomposites J. Phys.: Condens. Matter
 Robertson C G, Lin C J, Rackaitis M and Roland C M 2008 Inﬂuence of particle size and polymer–ﬁller coupling on viscoelastic glass transition of particle-reinforced polymers Macromolecules41 2727–31
 Sanctuary R, Baller J, Zielinski B, Becker N, Kruger J K, Philipp M, Muller U and Ziehmer M 2009 Inﬂuence of Al2O3 nanoparticles on the isothermal cure of an epoxy resin J. Phys.: Condens. Matter21 035118
 Schawe J E K 1995 A comparison of different evaluation methods in modulated temperature DSC Thermochim. Acta
 Tsagaropoulos G and Eisenberg A 1995 Direct observation of 2 glass transitions in silica-ﬁlled polymers—implications for the morphology of random ionomers Macromolecules28
 Tsagaropoulos G and Eisenberg A 1995 Dynamic–mechanical study of the factors affecting the 2 glass-transition behavior ofﬁlled polymers—similarities and differences with random ionomers Macromolecules28 6067–77
 Wetzel B, Rosso P, Haupert F and Friedrich K 2006 Epoxy nanocomposites—fracture and toughening mechanisms Eng. Fract. Mech.73 2375–98
 Yong V and Hahn H T 2004 Processing and properties of SiC/vinyl ester nanocomposites Nanotechnology15
 Zhao S, Schadler L S, Duncan R, Hillborg H and Auletta T 2008 Mechanisms leading to improved mechanical performance in nanoscale aluminaﬁlled epoxy Compos. Sci. Technol.68 2965–75
 Zunjarrao S C and Singh R P 2006 Characterization of the fracture behavior of epoxy reinforced with nanometer and micrometer sized aluminum particles Compos. Sci. Technol.